In this study, Fe3O4/graphene nanocomposite was synthesized through a liquid-phase co-precipitation method and characterized using X-ray diffraction and Fourier transform infrared spectrometer. The synthetic Fe3O4/graphene was used as a heterogeneous catalyst to activate persulfate to efficiently degrade methylene blue (MB). The target pollutant MB can be degraded by sulfate radicals depending on several parameters including persulfate and Fe3O4/graphene concentrations, pH and reaction temperature. Within 120 min of reaction time, almost 100% of 0.05 mM MB was removed by 1.5 mM persulfate in the presence of 150 mg/L of Fe3O4/graphene at pH = 6.0 and 25 °C. The degradation of MB was found to follow the pseudo-first-order kinetic model. The Fe3O4/graphene has much better stability and reusability than free Fe3O4 suggested by reuse tests. The results demonstrate that Fe3O4/graphene activated persulfate is a promising technology for remediation of water pollution caused by organic contaminants.
In the last decade, advanced oxidation methods based on sulfate radicals (SO4–•, E0 = 2.6 V) have drawn considerable interest on account of the disposal of hazardous compounds in aqueous phase or soil due to its advantages, such as stability, simple operation, high efficiency and no secondary pollution (Tsitonaki et al. 2010).
Fe3O4 magnetic nanoparticles (Fe3O4 MNPs) have been used as a suitable heterogeneous catalyst for activating persulfate due to the relatively wide availability and specific structural, easy separation/reuse and environmental friendliness (Yan et al. 2011; Ruan et al. 2015; Zhao et al. 2015). However, Fe3O4 MNPs-based persulfate oxidation is limited by the relatively low catalytic activity, low utilization efficiency of oxidants, and incomplete degradation of organic compounds. Recently, some scholars reported that the stability, dispersibility and catalytic efficiency of Fe3O4 MNPs to persulfate or H2O2 could be improved by modifying their surface with polymers such as poly(3,4-ethylene-dioxythiophene) (Shin et al. 2008), humic acid (Niu et al. 2011), and polyhydroquinone (Leng et al. 2013).
As a monolayer of carbon atoms with a tight packing of honeycomb lattice, graphene has attracted immense research interest in nanotechnology in recent years (Geim & Novoselov 2007). Graphene can increase the charge transfer rate of electrons and the surface-adsorbed amount of chemical molecules through π–π interaction. As a result of its unique physical and chemical properties, graphene oxide (GO) has also been used for adsorbing dye from wastewater discharged from the textiles, printing, and tanning industries (Bradder et al. 2010). More recently, Fe3O4/GO and Fe3O4/graphene composites have sparked much interest in promoting transfer and adsorption properties (Wang et al. 2012; Yao et al. 2012). Nevertheless, to our knowledge, there has been no study of the Fe3O4/graphene composites for activating persulfate so far.
In this study, Fe3O4 MNPs were embedded onto graphene to act as an activator for persulfate generating SO4–• radicals to oxidize organic target pollutants. Methylene blue (MB) was chosen as the typical dye pollutant. The present work aimed at providing insight into the activating ability and feasibility of Fe3O4/graphene to enhance the decomposition of persulfate and then degrade MB.
MATERIALS AND METHODS
Natural graphite powder was purchased from Qingdao Chenyang Graphite Company, China. MB, FeCl3·6H2O, NaOH and K2S2O8 were purchased from Beijing Chemical Reagent Company (Beijing, China). All other chemicals were of analytical grade and used without further purification. Ultra-pure H2O (>18 MΩ/cm) was used in the experiments.
Preparation of GO
GO was prepared from graphite powder by using a modified Hummers method as described by Wang et al. (2012). In brief, graphite powder (10 g) and NaNO3 (7.5 g) was added with stirring into concentrated H2SO4 (98%, 300 mL) solution in which KMnO4 (40 g) was completely dissolved. After 3 days of vigorous stirring at room temperature, the mixture was added into 1 L of 1% H2O2 solution. Then, the mixture was filtered and washed with deionized water until the pH of the filtrate became neutral. To remove the residual salts and acids, the resulting black paste was subjected to dialysis for 1 week by re-dispersing in deionized water, and then the brown suspension was dried at 40 °C under vacuum. GO was obtained as a gray powder.
Preparation of Fe3O4/graphene
The Fe3O4/graphene nanocomposite was prepared by the solvothermal method (Ai et al. 2011). Typically, a certain amount of the as-prepared GO was completely dispersed in 70 mL ethylene glycol and the mixture was ultrasonicated for 3 h. Then, 1.4 g FeCl3·6H2O and 2.8 g sodium acetate were added into the above mixture. After 30 min of stirring at room temperature, the mixture was transferred into a Teflon stainless-steel autoclave and reacted at 200 °C for 6 h in an oven. Afterwards, the autoclave was taken out of the oven and cooled to room temperature. The obtained Fe3O4/graphene nanocomposite was thoroughly washed sequentially with ultrapure water and ethanol and vacuum-dried at 60 °C. The Fe3O4/graphene composites with different mass ratios of Fe3O4 to GO (1:0.5, 1:1, 1:2, 1:3, 1:5) were synthesized by varying the amount of GO.
X-ray powder diffraction (XRD) measurements were carried out with a Bruker D8 advance diffractometer (Bruker, Germany) with Cu Kα radiation from 5 to 70 ° at a rate of 0.2 °/s. Fourier transform infrared (FT-IR) spectra were obtained by the KBr method with a JIR-6500W FT-IR spectrometer (Nihon Denshi, Tokyo, Japan).
Performance study of the Fe3O4/graphene sample
The catalytic degradation experiments of MB were conducted in 250 mL conical flasks sealed with Teflon-lined screw caps under mechanical stirring at various temperatures. In a typical run, 5–25 mg of Fe3O4/graphene was added to the flasks containing 100 mL MB solution, followed by 20 min of stirring to reach the adsorption–desorption equilibrium. Then, the MB concentration was measured and taken as the initial concentration. Prior to each experiment, Fe3O4/graphene was sonicated for 10 min to obtain well-suspended particles. The reaction was initiated immediately by adding 13.5–81 mg K2S2O8. To optimize the treatment efficiency of MB degradation by K2S2O8 using Fe3O4/graphene as the activator, five activator dosage gradients (50, 100, 150, 200 and 250 mg/L), six oxidant dosage gradients (0.5, 1.0, 1.5, 2.0, 2.5 and 3.0 mM), five pH gradients (pH 4.0, 5.0, 6.0, 7.0 and 8.0), and five temperature gradients (15, 25, 35, 45 and 55 °C) were chosen to study their effects on the degradation efficiency. The solution pH was adjusted by using NaOH (1.0 M) or H2SO4 (1.0 M) solution. At selected time intervals, 2 mL of samples were collected from each replicate flask, and immediately filtered through 0.22 μm membrane. After filtration, 0.2 mL of 0.2 mM Na2SO3 solution was added into the filtrate to quench any residual sulfate radicals and hydroxyl radicals (Tan et al. 2014).
The used activator was collected by a permanent magnet, rinsed with Milli-Q water several times, dried at 80 °C for 12 h, and then used for initiating the second treatment in the same reaction system. The recycled activator would be reused for at least three other cycles.
The concentrations of MB in the solution were determined using the spectrophotometeric method at 664 nm. The amount of total iron (Fe2+ plus Fe3+) leaching from the activator into reaction solutions was monitored by atomic absorption spectroscopy (model Z-2000; Hitachi, Tokyo, Japan). In this study, all oxidation tests were performed in triplicate, and results represented the means of three parallel experiments.
RESULTS AND DISCUSSION
Figure 1(b) shows the FT-IR spectra of GO and Fe3O4/graphene. Fe3O4/graphene and GO both show the O–H stretching vibration adsorption peak at 3,430 cm−1. The bands at 1,628 and 1,632 cm−1 are associated with stretching of the C = O bond of carboxyl groups. The band at 1,380 cm−1 is the C = O stretching vibration peak of carboxyl and carbonyl. The band at 1,060 cm−1 is ascribed to the C–O stretching vibration of the epoxy group and alkoxy (Chandra et al. 2010). The band at 571 cm−1, which only presents in the FT-IR spectrum of Fe3O4/graphene, can be ascribed to lattice absorption of iron oxide. Additionally, a new band is observed at 1,568 cm−1 for Fe3O4/graphene, which is attributed to the asymmetric vibration of COO−. This is the evidence for plenty of COO– coordinated with ferric ion (Ge et al. 2007). In comparison with GO, Fe3O4/graphene shows a dramatic decrease in the intensity of adsorption bands of oxygen-containing functional groups, indicating that GO has been substantially reduced.
Effect of Fe3O4/GO mass ratio on degradation effectiveness
Effect of Fe3O4/graphene dosage on degradation effectiveness
To check the catalytic activity of Fe3O4/graphene composite on persulfate for the degradation of MB, a set of experiments was conducted for 120 min with the Fe3O4/graphene dosage ranging from 50 to 250 mg/L. The experiments were run with an initial MB concentration of 0.05 mM, fixed persulfate concentration of 1.5 mM, pH 6.0 and at 25 °C.
Effect of persulfate concentration on degradation effectiveness
Oxidant concentration has an important influence on the treatment process efficiency and operational costs. To elucidate the role of persulfate concentration on the degradation of MB, a set of experiments were conducted for 120 min with the persulfate concentration ranging from 0.5 to 3.0 mM. The experiments were run with an initial MB concentration of 0.05 mM, fixed Fe3O4/graphene dosage of 150 mg/L, pH 6.0 and at 25 °C.
Effect of initial solution pH on degradation effectiveness
The influence of initial solution pH was investigated on the MB degradation in the system of 0.05 mM MB + 1.5 mM K2S2O8 + 150 mg/L Fe3O4/graphene.
Similar results were also reported in sulfamonomethoxine degradation by Fe3O4 activated persulfate system (Yan et al. 2011). In aqueous solution, MB and persulfate are presented as negative ions, thus increasing solution pH would increase the amount of negative surface charge on the activator. This would inhibit the static interactions between Fe3O4/graphene and MB or persulfate, and consequently result in a slower rate of reactive species production and dye degradation. Moreover, self-dissociation of persulfate mainly through non-radical pathways increases with an increment in solution pH, which would additionally reduce the degradation efficiency of the target pollutants (Rastogi et al. 2009).
Effect of temperature on degradation effectiveness
It is known that the oxidation capability of persulfate is moderate at room temperature, and the formation rate of SO4–• is pronounced at higher temperatures due to the increased thermal decomposition of persulfate (Kolthoff & Miller 1951). To investigate the influence of temperature on persulfate oxidation of aqueous MB solution (0.05 mM), a series of experiments were conducted at an initial persulfate concentration of 1.5 mM, an initial Fe3O4/graphene dosage of 150 mg/L, and an initial pH of 6.0 in the temperature range of 15–55 °C.
Stability and reusability of Fe3O4/graphene
To evaluate the stability of the Fe3O4/graphene activator, the leaching of Fe2+ and Fe3+ was determined over time during persulfate oxidation of MB. Under the experimental conditions, Fe2+ ions leached were rapidly oxidized to Fe3+ ions by the radicals, thus only Fe3+ ions were detected and presented. As shown in Figure 7(b), as the cycle time increased, the concentration of Fe3+ leached increased gradually but was always below the legal limits of USA and China (300 μg/L). Moreover, the concentration of Fe3+ was lower in the case of Fe3O4/graphene than in the case of Fe3O4. This suggests that the Fe3O4/graphene activator was stable during the catalytic reactions.
In the present study, Fe3O4/graphene nanocomposite was prepared and characterized by XRD and FT-IR. The effects of different conditions on the degradation of MB by Fe3O4/graphene activated persulfate were investigated. Results show that Fe3O4/graphene could effectively catalyze persulfate to degrade MB. Within 120 min of reaction time, almost 100% of 0.05 mM MB was removed at an initial persulfate concentration of 1.5 mM in the presence of 150 mg/L of Fe3O4/graphene at pH = 6.0 and 25 °C. Under the experimental conditions, the reactions followed the pseudo-first-order kinetics model. Fe3O4/graphene exhibited good stability and reusability, and it can be reused several times by separation from solution with employment of an external magnet. The Fe3O4/graphene showed better catalytic performance and excellent reusability compared to free Fe3O4. During the reaction, the activator was stable without significant leaching of iron into water.